Temperature-dependent studies of a new two-dimensional cadmium dicyanamide framework exhibiting an unusual temperature-induced irreversible phase transition into a three-dimensional perovskite-like framework.
Mączka, Mirosław; Gągor, Anna; Ptak, Maciej; Stefańska, Dagmara; Sieradzki, Adam; Physical chemistry chemical physics : PCCP 20 (2018) 29951–29958; doi:10.1039/c8cp06190d

data_7231872
_publ_section_title
;
 Temperature-dependent studies of a new two-dimensional cadmium
 dicyanamide framework exhibiting an unusual temperature-induced
 irreversible phase transition into a three-dimensional perovskite-like
 framework.
;
_journal_issue                   47
_journal_name_full               'Physical chemistry chemical physics : PCCP'
_journal_page_first              29951
_journal_page_last               29958
_journal_paper_doi               10.1039/c8cp06190d
_journal_volume                  20
_journal_year                    2018
_chemical_formula_sum            'C18 H28 Cd N10'
_chemical_formula_weight         496.90
_space_group_crystal_system      tetragonal
_space_group_IT_number           114
_space_group_name_Hall           'P -4 2n'
_space_group_name_H-M_alt        'P -4 21 c'
_symmetry_space_group_name_Hall  'P -4 2n'
_symmetry_space_group_name_H-M   'P -4 21 c'
_atom_sites_solution_hydrogens   geom
_audit_creation_method           SHELXL-2014/7
_audit_update_record
;
2018-09-24 deposited with the CCDC.
2018-11-19 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   16.2757(2)
_cell_length_b                   16.2757(2)
_cell_length_c                   17.5837(4)
_cell_measurement_reflns_used    7166
_cell_measurement_temperature    297(2)
_cell_measurement_theta_max      28.3131
_cell_measurement_theta_min      2.7525
_cell_volume                     4657.89(13)
_computing_cell_refinement
;
CrysAlisPro, Oxford Diffraction Ltd.,
Version 1.171.34.36 (release 02-08-2010 CrysAlis171 .NET)
(compiled Aug  2 2010,13:00:58)
;
_computing_data_collection
;
CrysAlisPro, Oxford Diffraction Ltd.,
Version 1.171.34.36 (release 02-08-2010 CrysAlis171 .NET)
(compiled Aug  2 2010,13:00:58)
;
_computing_data_reduction
;
CrysAlisPro, Oxford Diffraction Ltd.,
Version 1.171.34.36 (release 02-08-2010 CrysAlis171 .NET)
(compiled Aug  2 2010,13:00:58)
;
_computing_structure_refinement  'SHELXL-2014/7 (Sheldrick, 2014)'
_diffrn_ambient_temperature      297(2)
_diffrn_detector_area_resol_mean 8.4350
_diffrn_measured_fraction_theta_full 0.995
_diffrn_measured_fraction_theta_max 0.968
_diffrn_measurement_device_type  'Xcalibur, Sapphire1, long nozzle'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'Enhance (Mo) X-ray Source'
_diffrn_radiation_type           'Mo K\a'
_diffrn_radiation_wavelength     0.7107
_diffrn_reflns_av_R_equivalents  0.1696
_diffrn_reflns_av_unetI/netI     0.1385
_diffrn_reflns_Laue_measured_fraction_full 0.995
_diffrn_reflns_Laue_measured_fraction_max 0.968
_diffrn_reflns_limit_h_max       21
_diffrn_reflns_limit_h_min       -20
_diffrn_reflns_limit_k_max       21
_diffrn_reflns_limit_k_min       -21
_diffrn_reflns_limit_l_max       22
_diffrn_reflns_limit_l_min       -19
_diffrn_reflns_number            47231
_diffrn_reflns_point_group_measured_fraction_full 0.997
_diffrn_reflns_point_group_measured_fraction_max 0.969
_diffrn_reflns_theta_full        25.000
_diffrn_reflns_theta_max         28.375
_diffrn_reflns_theta_min         2.758
_exptl_absorpt_coefficient_mu    0.962
_exptl_absorpt_correction_T_max  1.00000
_exptl_absorpt_correction_T_min  0.85428
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details
;
CrysAlisPro, Oxford Diffraction Ltd.,
Version 1.171.34.36 (release 02-08-2010 CrysAlis171 .NET)
(compiled Aug  2 2010,13:00:58)
Empirical absorption correction using spherical harmonics,
 implemented in SCALE3 ABSPACK scaling algorithm.
;
_exptl_crystal_colour            colourless
_exptl_crystal_density_diffrn    1.417
_exptl_crystal_description       prism
_exptl_crystal_F_000             2032
_exptl_crystal_size_max          0.31
_exptl_crystal_size_mid          0.20
_exptl_crystal_size_min          0.15
_refine_diff_density_max         0.678
_refine_diff_density_min         -0.571
_refine_diff_density_rms         0.087
_refine_ls_abs_structure_details
;
 Refined as an inversion twin.
;
_refine_ls_abs_structure_Flack   0.41(11)
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.083
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     249
_refine_ls_number_reflns         5595
_refine_ls_number_restraints     20
_refine_ls_restrained_S_all      1.082
_refine_ls_R_factor_all          0.1942
_refine_ls_R_factor_gt           0.0797
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.0230P)^2^+2.8000P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1098
_refine_ls_wR_factor_ref         0.1387
_reflns_Friedel_coverage         0.821
_reflns_Friedel_fraction_full    0.998
_reflns_Friedel_fraction_max     0.970
_reflns_number_gt                2683
_reflns_number_total             5595
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            c8cp06190d2.cif
_cod_data_source_block           Phase_tetra
_cod_depositor_comments
'Adding full bibliography for 7231870--7231872.cif.'
_cod_original_cell_volume        4657.89(16)
_cod_database_code               7231872
_shelx_shelxl_version_number     2014/7
_shelx_res_checksum              907